Marginal distortion of thermally incompatible metal ceramic crowns with overextended margins.
OBJECTIVE
The present study tested the hypothesis that metal ceramic crowns with a varying axial height are more susceptible to marginal distortion during mechanical and thermal processing treatments than crowns with a uniform axial height.


METHODS
Copings of Pd-Cu-Ga alloy with buccal margin extensions of 0, 1.5, and 3.0 mm were prepared. Oxidized copings were veneered with experimental opaque porcelain with a mean thermal contraction coefficient (25 degrees C to 500 degrees C) that was either 2.1 ppm/degree C below (delta alpha = +2.1 ppm/degree C) or 0.1 ppm/degree C above (delta alpha = -0.1 ppm/degree C) that of the alloy. Nine groups of six specimens each were prepared for analysis. Eighteen copings from these 54 specimens were used as porcelain-free controls. All specimens were subjected to a 10-step procedure including grinding, oxidation, firing of four opaque porcelain layers (O1: 0.15 mm; O2: 0.15 mm; O3: 0.5 mm; O4: 0.5 mm), glazing, abrasive blasting for 15 seconds, removal of ceramic by dissolution in hydrogen fluoride, and a postannealing treatment. The control specimens were also subjected to this procedure with the exception of the firing of four layers of porcelain, which were not applied. Marginal gap width was determined using a measuring microscope at a magnification of 30x.


RESULTS
Analysis of variance revealed a significant difference in mean gap width as a function of axial length. The largest gap change was associated with a 3.0-mm buccal extension and the negative mismatch condition (delta alpha < 0).


CONCLUSIONS
Marginal distortion of crowns decreases as the axial length becomes more uniform. Analysis of crown distortion based on differences in the mean contraction coefficients of metal and porcelain alone is not recommended because it ignores the effects of metal grinding, metal sandblasting, and transient stress.
Department of Fixed Prosthodontics, School of Dental Medicine, Tsurumi University, Yokohama, Japan.
Y
Y
Nakamura
K J
KJ
Anusavice
D000704:Analysis of Variance; D003442:Crowns; D000044:Dental Abutments; D003722:Dental Alloys / Q000737:chemistry*; D018772:Dental Marginal Adaptation; D003776:Dental Porcelain / Q000737:chemistry; D017267:Dental Prosthesis Design / Q000706:statistics & numerical data; D003799:Dental Stress Analysis; D008422:Materials Testing; D016876:Metal Ceramic Alloys / Q000737:chemistry*; D008669:Metallurgy; D010165:Palladium; D013816:Thermodynamics
D003722:Dental Alloys; D016876:Metal Ceramic Alloys; D003776:Dental Porcelain; D010165:Palladium